Preparation of (pomegranate peel polystyrene) composites and study their optical properties
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201322Preparation of (Pomegranate Peel- Polystyrene) Composites andStudy their Optical PropertiesFalah Ali Jasim1, Ahmed. Hashim2, Angham.G.Hadi 3, Farhan Lafta4, Saba R. Salman5and Hind Ahmed61,4Ministry of Science and Technology, Iraq2,3,5,6Babylon University, Iraq2E-Mail: firstname.lastname@example.orgE-Mail: email@example.comAbstractIn this work, samples of pure polystyrene and polystyrene (PS) doped with (pomegranate peel) were preparedusing casting method .The effect of addition of pomegranate peel (PP) concentration on optical properties ofpoly styrene have been studied in the wavelength range (200-800)nm. The absorption coefficient, energy gap,refractive index and extinction coefficient have been determined. The results show that the optical constantschange with increase of PP concentration.Key words: polymer , Polystyrene, pomegranate peel, Optical properties, absorbance.1.IntroductionOptical polymers have attracted considerable attention in recent years because of their important industrialapplications. The study of phase separation in thin films of binary mixtures is commercially important for theeffective production of various coatings and films, including dielectric layers, photographic materials and paintsystems. While film of polymer blends often exhibit more desirable characteristics than individual homopolymers, most blend components are also highly incompatible with each other and will demix and phase-separate. The degree of separation in blends will greatly affect the resulting morphology, which can have adverseaffects on the properties of the resulting film[1-3]. One method often used to improve properties of a speciﬁcconductive polymer is to prepare composites using selective inorganic oxides such as SiO2, TiO2, andzeolite [4-6]. Some other useful methods are the prepa-ration of blends, composites, or copolymers ofpoly thiophene using insulating polymers as processing aid [7–13]. Ideally, such composites would possessa combination of the outstanding process ability and thermal stability characteristic of the insulating polymersand the electrical conductivity and optical properties of the conduct-ing polymers, resulting in aninteresting advanced material. Among insulating polymers, polystyrene (PS) and poly methyl methacrylate(PMMA) show good and mechanical properties. PS and PMMA are chemically stable thermoplasticsthat are designed for applications requiring optical transparency and outstanding mechanical behavior aswell as good process ability.The objective of this study was to help in understanding the effect of different concentrations of (PP) on theoptical properties of (PS).2.Experimental PartThe polymer (PS) was dissolved in chloroform by using magnetic stirrer in mixing process to gethomogeneous solution. The weight percentages of PP are (2, 4 ,6 wt%) were added and mixed for 10 minute toget more homogenous solution , after which solution was transferred to clean glass Petri dish of (5.5cm) indiameter placed on plate form. The dried film was then removed easily by using tweezers clamp. The polymersystems were evaluated spectra photo metrically by using UV/160/Shimadzu spectrophotometer.3.Results & Discussion3.1 The absorbance of composites
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201323Fig(1) shows the relationship between absorbance of PS-PP composite with wave length, from the figure it wasappeared that the absorbance tends to decrease with the wavelength increasing.Fig(2) shows the optical absorption spectrum of composite for different impurities quantities, it was found thatthe composite have a low absorption coefficient at a small photon energy then increase at different ratesdependence on the composite structure. The pure sample had low absorption coefficient this may be as a result oflow crystalinity.0501001502002503003500 1 2 3 4 5 6 7Photon energy(eV)pure2 wt.%4 wt.%6 wt.%α(cm)-1FIG. 2 The Absorption Coefficient Of PS-PP Composite With Photon Energy00.511.522.533.54200 300 400 500 600 700 800Wavelength(nm)Absorbancepure2 wt.%4 wt.%6 wt.%FIG.1 The relationship between absorbance and the wave length of PS-PP
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201324Fig (3) and Fig(4) represented the direct transition , the energy gab values dependence in general on the crystalstructure of the composites and on the6arrangement and distribution way of atoms in the crystal lattice .3.3Refractive Index and Extinction CoefficientFig. (5 ) shows the variation of refractive index(n) with of the composite with a given photon energy thevalues increase exponentially with increasing photon energy . This increase indicates that the electromagneticradiation passing through the material is faster in the low photon energy.Fig. (6) represent the variation of the extinction coefficient(k) with the incident photon energy in thisfigure the variation is simple in the low energy region while the variation increased in the high photon energyregion this behavior may be as a result to the variation of the absorption coefficient which leads to spectral0204060801001200 1 2 3 4 5 6 7Photon energy(eV)pure2 wt.%4 wt.%6 wt.%(αhυ)1/3(cm-1.eV)1/3FIG.4 the relationship between (αhυ)1/3(cm-1.eV)1/3and photon energy of PS-PP composites010020030040050060070080090010000 1 2 3 4 5 6 7Photon energy(eV)pure2 wt.%4 wt.%6 wt.%(αhυ)1/2(cm-1.eV)1/2FIG.3 relationship between (αhυ)1/2(cm-1.eV)1/2and photon energy of PS-PP composites.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201325deviation in the location of the charge polarization at the attenuation coefficient due to the loses in the energy ofthe electron transition between the energy bands .184.108.40.206.8220.127.116.11.80 1 2 3 4 5 6 7photon energy(eV)npure2 wt.%4 wt.%6 wt.%FIG.6 The Relationship Between Refractive Index For (PS-PP) Composite WithPhoton Energy1.E-081.E-071.E-061.E-051.E-040 1 2 3 4 5 6 7k pure2 wt.%4 wt.%6 wt.%photon energyFIG.5 The Extinction Coefficient Of PS-PP Composite With Various PhotonEnergy
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 2013263.4dielectric constantFig.(7) & (8) represent the real and imaginary parts of the dielectric constant respectively in the real part thevariation is very clear spatially in the high impurities concentration this may be due to the no resonance betweenthe frequencies of the incident photon energy (electromagnetic and the induced dipoles in the composite), whilein the imaginary part there is an absorption to the energy of the incident photon energy, so the variation nearlyconstant until it reaches to the high photon energy . The pure composite shows the smaller variationConclusions• The absorbance is very large in the uv, region. The absorption coefficient is smaller and stable in thelow photon energy.• The absorption and (k) will increase as a result of the scattering centers in the composites. The values ofthe refractive index(n) of the composites increase exponentially with increasing photon energy .• The real and imaginary dielectric constant shows the exponential increase with increasing the incidentphoton energy.1.E-071.E-061.E-051.E-040 2 4 6 8photon energy(eV)pure2 wt.%4 wt.%6 wt.%ε2FIG. 8 The Variation Of Imaginary Part Of Dielectric Constant Of PS-PP CompositeWith Photon Energy01234567890 1 2 3 4 5 6 7photon energy(eV)pure2 wt.%4 wt.%6 wt.%ε1FIG.7 The Variation Of Real Part Of Dielectric Constant PS-PP With PhotonEnergy
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.18, 201327References Ade H, Zhang X, Cameron S, Costello C, Kirz J. and Williams S, Science 258:972 (1992). Ade H and Hsiao B, Science 262:1427 (1993).[ 3] Ade H, Trends Polym Sci :58, 66 (1997). J. Stejskal, P. Kratochvil, S.P. Armes, S.F. Lascelles, A. Riede, .Helmstedt, I. Krivka, Polyanilinedispersions. 6. Stabilization by colloidal silica particles, Macromolecules 29 (1996) 6814–6819. N. Hebestreit, J. Hofmann, U. Rammelt,W. Plieth, Physical and electrochemical characterization of nanocomposites formed from polythiophene and titanium-dioxide,Electro chim. Acta 48 (2003) 1779–1788 N. Ballav, MBiswas, A conductive composite of polythiophene with 13X-zeolite, Mater. Sci. Eng. B 129(2006) 270–272. M.A. Monedero, G.S. Luengo, S. Moreno, F. Ortega, R.G. Rubio, M.G. Prolongo, R.M. Masegosa,Calorimetric and dielectric study of a blend ontaining aconductive polymer: poly(3-octylthiophene) +poly(ethylene-co-nylacetate),Polymer 40 (1999) 5833–5842. J. Jaczewska, A. Budkowski, A. Bernasik, I. Raptis, J. Raczkowska, D.Goustouridis, J. Rysz, M. Sanopoulou, Humidity and solvent effects in spin-coated polythiophene–polystyrene blends, J. Appl. Polym. Sci. 105 (2007)67–79. J. Jaczewska, A. Budkowski, A. Bernasik, E. Moons, J. Rysz, Polymer vs solvent diagram of ﬁlmstructures formed in spin-cast poly(3-alkylthiophene) blends,Macromolecules 41 (2008) 4802–4810. K. Kanemoto, K. Shishido, M. Sudo, I. Akai, H. Hashimoto, T. Karasawa,Concentration-dependence of photoluminescence properties in poly thiophenediluted in an inactive polymer matrix, Chem. Phys. Lett. 402 (2005)549–553. R.M. Masegosa, D. Nava, S. García, M.G. Prolongo, C. Salom, Thermal behavior of unsaturatedpolyester resins + poly(3-octylthiophene) blends, Thermo chim. Acta 385 (2002) 85–94. B. Sari, M. Talu, F. Yildirim, E.K. Balci, Synthesis and characterization of olyurethane/poly thiopheneconducting copolymer by electrochemical method,Appl. Surf.Sci. 205 (2003) 27–38. Özgün Aylin, Bekir Sari, Aysegül Uygun, H. Ibrahim Ünal, Cetin akanyildirim,Conductingcomposites and blends of polythiophene and poly oxymethy lene, Int. J. Polym. Anal. Charact. 14 (2009)469–480.